International Journal of Computational Engineering Research||Vol, 03||Issue, 5||www.ijceronline.com ||May ||2013|| Page 71Experimental Investigation of Multiwalled Carbon NanotubeReinforcement in the Metal Matrix Composites for High ValueFatigue LifeG.E.V.Ratna Kumar 1, P.N.S.Srinivas 21,Asst Prof (Department of mechanical engineering), Sri Vasavi institute of engineering & technology, JNTUK,INDIAAsst Prof (Department of mechanical engineering),Sri Vasavi institute of engineering & technology, JNTUK,INDIAI. INTRODUCTIONGlass fiber composites have high strength and low cost, but suffer from poor performance in fatigue.The underlying mechanisms in high-cycle fatigue failure of glass fiber composites are primarily related to ma-trix-dominated damage accumulation and growth that coalesce and propagate to the fibers resulting in ultimatefailure.Prior fatigue studies of continuous and aligned glass fiber composites have shown that high-cycle fatiguelife is dominated by fatigue cracking in the matrix that subsequently propagate and rupture the fibers. Once asignificant number of fibers fracture, the composite laminate fails shortly thereafter. Unlike in high moduluscarbon fiber composites, the low modulus of the glass fibers results in the imposition of high strains in thematrix leading to matrix fatigue failure . In these studies, failure was defined as the number of cycles when aprescribed loss of stiffness is attained. A recent review of fatigue theories is given in the following technicalmaterial. Stiffness reduction is an index of damage in composites and has been studied extensively boththeoretically and experimentally. However, crack propagation and the resulting loss in stiffness is only a grossoverall indicator of damage in composites. Damage can be generated well before microscopic-level crackinitiation and micro crack coalescence occurs. Other studies have focused on measuring the fracture energiesinvolved in crack propagation in composites, particularly in delamination fracture, a common failure mode .Such studies show that a single crack that propagates in the matrix or fiber/matrix interface in a composite isassociated with a low level of absorbed fracture energy.In typical composite laminate configurations designed to carry structural loads under cyclic conditions,carbon fiber composites show little degradation with load cycling compared to glass composites. Theexplanation for the low degradation rates for carbon composites lies in the fact that the higher modulus ofcarbon fiber results in a low level of cyclic strain imposed on the matrix. A critical strain in the matrixcorresponding to the fatigue strain of the matrix at the corresponding applied composite stress was identified asthe critical parameter in fatigue failure of the composite.In glass composites, the applied cyclic strain in thematrix exceeds the corresponding fatigue strain in the neat resin, while in higher modulus composites such ascarbon fiber composites; the applied cyclic strain in the matrix is below this critical value. Thus carboncomposites show little degradation with cycling and are accepted as having good fatigue strength. Thisexplanation has been verified recently on oriented rope CNT-reinforced epoxy composites which have highmodulus .ABSTRACTThe present work shows that the addition of small volume fractions of multi-walled carbonnanotubes (CNTs) to the matrix results in a significant increase in the high-cycle fatigue life. It isproposed that carbon nanotubes tend to inhibit the formation of large cracks by nucleating nano-scaledamage zones. In addition, the contribution to energy absorption from the fracture of nanotubesbridging across nano-scale cracks and from nanotube pull-out from the matrix are mechanisms thatcan improve the fatigue life. An energy-based model was proposed to estimate the additional strainenergy absorbed in fatigue. The distributed nanotubes in the matrix appear to both distribute damageas well as inhibit damage propagation resulting in an overall improvement in the fatigue strength ofglass fiber composites.KEYWORDS: carbon nanotubes, fatigue life, strain energy, metal matrix composites, thermosettingpolymers, epoxy resins, cyclic stresses.
Experimental Investigation Of Multiwalled…www.ijceronline.com ||May ||2013|| Page 72Other studies on the effect of CNTs on the fracture of the matrix polymer have shown that small additionsof CNTs (0.1wt%-0.2wt %) resulted in a 40% increase in the fracture toughness of the polymer . Microscopystudies show a very high density of nano-scale cracks in the matrix that are attributed to the improvement in thefracture toughness of the matrix polymer.In this work, the effect of carbon nanotubes on the life of structuralcomposites subjected to static and cyclic loading is studied and a mechanism for the observed behavior isproposed. Damage mechanisms in conventional composite laminates consist of the formation of micro-cracks inthe matrix that initiate and propagate under cyclic loading, eventually causing fiber failure and fracture of thecomposite.The addition of CNTs can be expected to decrease the scale of damage mechanisms by several ordersof magnitude resulting in an increase in the absorption of strain energy through the creation of a multitude offine nano-scale cracks. In addition, fiber bridging at the nanoscale increases energy absorption through theparticipation of nanotubes in the fracture process. This effect should increase the damage tolerance of thecomposite and make it more resistant to damage growth under cyclic loading. An energy-based model isproposed that attempts to describe the fatigue behavior of CNT / glass-fiber hybrid composites.We haveincorporated thermosetting (epoxy) polymers containing uniformly distributed nanofibers (CNTs) intoconventional glass fiber polymer composites. Our recent studies have established that these resins exhibit arelatively uniform distribution of the nanofibers in the polymer with little agglomeration and clumping. Hy-brid composite systems that contain CNTs, both under static and cyclic loading, examined through scanningelectron microscopy of the corresponding fracture surfaces exhibit failure modes that suggest the failuremechanism that is proposed here.II. EXPERIMENTAL ANALYSISII.I. Materials: The epoxy resin and hardener used was EPON 826 and Epikure 3234, respectively, bothmanufactured by Hexion Specialty Chemicals, Inc.(Houston, Texas, USA). The EPON 826 resin was blendedwith 1wt% of multi-walled carbon nanotubes by Nanoledge (Clapiers, France). The current CNT loading levelof 1wt% was selected for its promise to be large enough to change the mechanical behavior of the composites [7,9]and at the same time not reduce manufacturability due to an increase in polymer viscosity .The woven glassfiber was obtained from Hexcel (Fullerton, CA USA) designated Type 7500, a 0.28 mm thick plain weavefabric.II.II.Specimen processing: Both the CNT and non-CNT [0/90] fiber reinforced composites weremanufactured by wet lay-up, cured in a heated platen press held at 80 °C and 580 kPa for one hour, with a fibervolume fraction of 0.56. Aligned 24 X 200 mm tensile specimens were cut from the cured sheets. A 6.4 mmdiameter center hole was drilled in each specimen to localize damage. Aluminum tabs were bonded to the endsof the specimens to facilitate gripping. The specimens were aged for 10 d at 25 C before testing.II.III.Test methods: Specimens were tested to failure using an MTS (Eden Prairie, Minnesota, USA) 100kN servo-hydraulic testing machine retrofitted with a variable flow hydraulic supply digitally controlled by anInstron (Norwood, MA USA) Labtronic 8400 controller. National Instruments (Austin, TX USA) Lab VIEW v7was used to command the controller and perform data acquisition. Prior to fatigue testing, the monotonic tensilestrengths of both CNT and non-CNT composite samples were obtained.Both materials were tested in tension-tension fatigue at peak stresses of 70, 60, 45 and 30 percent of their monotonic strengths, all at a stress ratio (R)of 0.15. The loading frequency used was 3 Hz to eliminate sample heating. Representative failed specimenswere chosen and their fracture surfaces were excised and sputter-coated with a 2.5 nm layer of platinum using aBal-Tec (Blazers, Liechtenstein) Med 020 coater. The samples were imaged using a Hitachi (Tokyo, Japan) S-5000 cold field emission SEM with an accelerating voltage of 10 kV.III. RESULTS AND DISCUSSIONIII.I. Tension testing: Fig.1 shows the stress-strain responses from monotonic tensile tests conducted onthe neat resin with and without CNTs. No significant effect on the elastic modulus was observed. The maximumvalues of strain to failure, however, were somewhat higher in the CNT-containing resin samples withcorresponding slightly lower ultimate tensile strengths when compared with the unmodified resin. Thesechanges in mechanical behavior result in an increased toughness, or energy to fracture, for the neat resincontaining CNTs. Figs.2 and 3 show scanning electron micrographs (SEMs) of the fracture surfaces of the twomaterials. The CNT-containing resin shows a somewhat rougher fracture surface, which is in line with the in-crease in the fracture energy discussed above.
Experimental Investigation Of Multiwalled…www.ijceronline.com ||May ||2013|| Page 73Fig.4 shows the monotonic tensile fracture surface in the neat resin containing CNTs. While there isgenerally uniform distribution of the CNTs in the resin, a few randomly distributed clumps of nanotubes (seeinsert in Fig.4) were also observed indicating that some agglomeration was present. These agglomerated regionsare thought to be detrimental to strength as well as fatigue life .Fig.5 shows the fracture surface of a hybrid CNTcomposite showing pull-out of the nanotubes from the matrix (small holes and larger protruding tubes in thefigure). Smaller protruding sections of nanotubes seen in this micrograph may indicate that nanotubes were alsofractured with the matrix. A single hole (white arrow) corresponds to a tube that was pulled out from this sur-face. It is this process of nanotube pullout and nanotube fracture that is believed to contribute to the increasedfracture resistance as well as significantly improved fatigue life (see below) in the hybrid CNT composites.Fig.1 Tensile stress-strain responses of neat resin with and without 1wt% of CNTsFig.2 Fracture surface of neat epoxy matrixIII.II. Fatigue life: Fatigue life data for glass fiber-epoxy composites (three samples per point) with andwithout the addition of 1wt% of carbon nanotubes are shown in Fig.6. A significant increase in the number ofload cycles to failure for each loading case was observed for the samples that contained the CNTs. The observedincrease in life occurs at lifetimes greater than about 104 cycles. In this high cycle regime, much of the loadcycles are employed for the nucleation and growth of micro cracks [1,2]. Table 1 compares the fatigue lifetimesfor glass fiber composites with and without carbon nanotubes (CNTs). The improvement in fatigue life with theaddition of CNTs increases as the applied cyclic stress is reduced, making the effect most pronounced at highcycles. At a cyclic stress of 44 Mpa, the addition of 1wt% of CNTs results in almost a 3 times improvement inthe fatigue life.Fig.3 Fracture surface of the CNT-modified epoxy matrix
Experimental Investigation Of Multiwalled…www.ijceronline.com ||May ||2013|| Page 74Fig.4 SEM image showing CNT distribution and an agglomerated region containing entangled carbon nanotubesFig.5 SEM image of fracture surface of glass fiber composite containing carbon nanotubes showing fracturedand pulled-out CNTs; the arrow points at a hole from which a nanotube was pulled outFig.6 Applied cyclic stress versus the number of cycles to failure of glass fiber-epoxy laminates with andwithout the addition of 1wt% of carbon nanotubesIn the composites containing nanotubes, it is believed their presence results in a very large number ofnucleating sites for cracks to be initiated and grow. Furthermore, it is believed for a given level of strain energy,a large density of nanoscale cracks will grow more slowly than the lower density of micro cracks present incomposites not containing CNTs.
Experimental Investigation Of Multiwalled…www.ijceronline.com ||May ||2013|| Page 75The result is an increase in the number of cycles required for growth and coalescence which means thathigh-cycle fatigue life is enhanced. In addition, nanoscale crack bridging by nanotubes will result inparticipation of the nanofibers in the fracture process thereby increasing the fracture energy required for crackpropagation, further delaying failure.III.III. Fracture surface analysis: High resolution scanning electron micrographs of the fracture surface of aglass fiber composite sample containing CNTs are shown in Fig.7. Both micrographs are from the samelocation; the micrograph on the right shows the scale of the carbon nanotubes relative to the fractured glass fiberon the left. Pull-out and fracture of carbon nanotubes were observed in the hybrid composite similar to themechanisms observed in the neat resin/CNTs fracture surface (Fig.5). Additionally, Fig.7 demonstrates theability of the CNTs to penetrate between glass fibers, further validating the proper dispersion of CNTs in thepolymer .III.IV.Differential energy model: A study of the electron micrographs of the fracture surfaces indicates thatthe primary difference in the fracture behavior of the traditional glass-fiber composites and the behavior of theCNT/glass-fiber hybrid composites from a mechanistic standpoint is the existence of broken and pulled-outnanotubes at the fracture surfaces within the hybrid epoxy matrix. It is proposed that these nano-scale processesin the hybrid composites results in an absorption and dissipation of strain energy which retards the growth ofmatrix micro cracks thereby extending the fatigue life.Fig.7 Fatigue fracture surface of glass fiber composite laminate containing 1wt% of carbon nanotubes in thematrix.The higher magnification micrograph on the right shows the carbon nanotubes in the matrix surrounding thefractured glass fiber shown at lower magnification on the leftIn the proposed model, individual CNTs are assumed to be evenly distributed and randomly oriented inthree dimensions within the epoxy matrix. This assumption facilitates the establishment of the micrometer-scalestatistical representative volume element. The bond between the nanotubes and the surrounding epoxy matrix isassumed to consist exclusively of van der Waals forces [13-15]. Due to the lower transverse coefficient ofthermal expansion (CTE) in the CNTs relative to the polymer matrix, the CTE mismatch following curing atan elevated temperature results in a compressive radial pre-stress on the nanotubes at room temperature.
Experimental Investigation Of Multiwalled…www.ijceronline.com ||May ||2013|| Page 76This gives rise to a frictional shear stress, Ԏp that resists nanotube pull-out. It is also believed that acertain degree of interlocking between the CNTs and the matrix may contribute to Ԏp . Nanotubes arepresumed to pull-out from the matrix unless they cross the fracture plane at a critical angle, φ that causes thetubes to fracture instead of pull out. The angle at which the behavior transitions from pull-out to fracture, φc, ispresumed to be related to the rate at which the two halves of the fracture surface are separated under cycling.This concept is presented in Fig.8.Fig.8 Observed behavior of individual CNTs at the fracture surfaceIII.V. Matrix fracture energy relation: General relations describing the potential energy losses in the elasticmatrix of a composite are developed for both the traditional composite and the CNT hybrid composite followingthe methods used for fracture in reinforced ceramics by Budiansky, et al. In the case of the traditionalcomposite, these losses are due to the creation of matrix cracks. Similarly, in the hybrid composite, these lossesgo toward the creation of matrix cracks, frictional sliding at The CNT/matrix interface during CNT pulls-out,and fracture of CNTs. The development of the energy relations for the two cases proceeds in parallel until theinclusion of the terms corresponding to the frictional sliding and fracture of CNTs. Throughout the derivation,symbols corresponding to the traditional composite case will be natural (X, Y), whereas those corresponding tothe hybrid composite case will be accented (X˜, Ỹ). Fig.9 presents the three states of interest in both cases.State(0) corresponds to a free body of volume V and surface ST, not subjected to any external loads, and exhibitingno displacements or strains, containing some internal stress distribution σ0. State (1) corresponds to the samebody, with applied tractions T, which result in a stress distribution σ1, displacements u1, and correspondingstrains ε1. With no change in the surface tractions T, state (2) has undergone some internal cracking resulting incrack surface SC, and new values of stress distribution σ2, displacements u2, and strains ε2. Similarly, forthe case of the hybrid composite matrix, state (õ) corresponds to a free body of volume Ԏand surface ԎT, notsubjected to any external loads, exhibiting no displacements or strains, containing some internal stressdistribution σ̃0. State (1̃) corresponds to the same body , with applied tractions T̃ , which result in a stressdistribution σ̃1, displacements ũ1, and corresponding strains ε̃1. With no change in the surface tractions T̃ , state(2̃) has undergone some internal cracking resulting in new crack surface S̃C, frictional sliding due to pull-out atthe new CNT / matrix interfacial surface S̃P, fracture of CNTs creating new CNT surface S̃ F, and new values ofstress distribution σ̃2, displacements ũ2, and strainsε̃2.The constitutive relations relating stress to strain in the two cases areε = M (σ－σ0) (1)For the traditional glass-fiber composite and:ε̃= M̃ (σ̃－σ̃0) (2)For the CNT/glass-fiber hybrid composite, where M and M̃ are the elastic compliances for the two cases.For the case of the traditional composite, the potential energy in each of the three states respectively can bedescribed as in  by:Π0＝1/2∫vσ0: M (σ0) D (3)Π1＝1/2∫vσ1: M (σ1) dV－∫STT·u1dV (4)Π2＝1/2∫vσ2: M (σ2) dV－∫STT·u2dV (5)Where, the volume integral describes the stored elastic energy and the surface integral describes thework done at the surface of the body by the applied tractions. Taking the compliance to be a constant,1: M (σ2) ＝σ2: M (σ1)The change in potential energy of the body due to the internal cracking is found to be:Π1－π2＝1/2∫v (σ1＋σ2):M (σ1―σ2) dV―∫ST T· (u1―u2) ds (6)Equating the external virtual work of the traction T over the displacement u1－u2 to the internal virtual workcorresponding to the internal stress, σ2 over the strain M (σ1－σ2), we have∫STT· (u1－u2) dS=∫vσ2: M (σ1―σ2) dV (7)
Experimental Investigation Of Multiwalled…www.ijceronline.com ||May ||2013|| Page 77Combining Eqs. (1), (6) and (7) gives us the general form for potential energy loss due to matrixcracking, from state (1) to state (2):π1－π2=1/2∫v (σ1―σ2): (ε1―ε2) dV (8)Derivation of the potential energy loss in the case of an elastic body containing frictional sliding andfiber breakage, in our case due to nanotube pull-out and the fracture of CNTs, proceeds much the same asbefore, up until the calculation of the virtual work. For completeness, the potential energy equation for thesecond case takes the exact form as its predecessor, Eq. (6), but with accented rather than natural notation:Thedifference in the derivation of the energy relations in the hybrid matrix case is the two additional internal virtualwork terms corresponding to the frictional sliding and fiber breakageIV. CONCLUSIONSThe addition of 1wt% of CNTs to the polymer matrix of glass fiber-epoxy composite laminatesimproved their high-cycle fatigue lifetimes significantly. Tensile tests on neat resin (without glass fibers)specimens showed no effect on the elastic modulus when CNTs were added. However, there was a slightincrease in the strain to failure and corresponding higher toughness relative to the unmodified resin. Highresolution scanning electron microscopy of the neat resin specimens after tensile fracture revealed somewhathigher surface roughness in the CNT-modified resin. Inspection of the composite specimens tested in fatigueshowed carbon nanotubes that were either pulled out of the resin matrix or fractured, suggesting energy-absorbing mechanisms that may be responsible for the increase in the fatigue life observed. These include thecreation of a much larger density of nucleation sites for fatigue crack initiation in the epoxy matrix as well aspossible crack bridging by the carbon nanotubes. Both mechanisms can result in a significant increase in crackenergy absorption during fatigue crack initiation, coalescence and propagation, resulting in the observedincrease in the fatigue life when carbon nanotubes are added.The energy based model presented here takes advantage of the even distribution and randomorientation of the large numbers of CNTs in the polymer matrix and uses this as a basis for establishing amicrometer-scale representative volume element with homogenized material properties that reflect themechanistic behavior of the entire population of CNTs it contains. Energy relations are developed for thishomogenized CNT / epoxy system in parallel with the neat epoxy matrix in order to establish the energeticdifferences, or differential energy, in the formation and propagation of cracks within their bodies.This studyshows that the addition of small fractions of carbon nanotubes to glass fiber composites can result in asignificant increase in their fatigue life, making glass fiber composites more useful in applications involvinghigh-cycle fatigue.REFERENCES Dharan CKH. Fatigue Failure Mechanisms in a Unidirectionally Reinforced Composite Material [M]. ASTM Spec. Tech. Publ.,1975, 569: 171 Dharan CKH. Fatigue Failure in Graphite Fibre and Glass Fabre- polymer Composites [J]. J. Mater. Sci., 1975, 10: 1 655 Hahn HT, Kim RY. Fatigue Behavior of Composite Laminate [J]. J. Compos. Mater, 1976, 10: 156 Degrieck J, Van Paepegem W. Fatigue Damage Modeling of Fiber-reinforced Composite Materials: Review [J]. Appl.Mech. Rev., 2001, 54(4): 279 Saghizadeh H, Dharan CKH. Delamination Fracture Toughness of Graphite and Aramid-epoxy Composites [J]. J. Eng. Mater.Tech.: Trans. ASME, 1986, 108(4): 290 Ren Y, Lil F, Cheng HM, et al. Fatigue Behaviour of Unidirectional Single-walled Carbon Nanotube ReinforcedEpoxy Composite under Tensile Load[J]. Adv. Compos. Lett., 2003, 12(1): 19 Ganguli S, Aglan H. Effect of Loading and Surface Modification of MWCNTs on the Fracture Behavior of Epoxy Nancomposites [ J]. J. Reinforc. Plast. Compos. 2006, 25(2): 175 Grimmer CS, Dharan CKH. High-cycle Fatigue of Hybrid Carbon Nanotube/Glass Fiber/Polymer Composites [J]. J. Mater. Sci.,2008, 43: 4487 Gojny FH, Wichmann MHG, Fiedler B, et al. Influence of Nano-modification on the Mechanical and Electrical Properties ofConventional Fibre-reinforced Composites [J]. Compos. A, 2005, 36: 1525 Kim JA, Seong DG, Kang TJ, et al. Effects of Surface Modification on Rheological and Mechanical Properties ofCNT/Epoxy Composites [J]. Carbon, 2006, 44: 1898 Wong M, Paramsothy M, Xu XJ, et al. Physical Interactions at Carbon Nanotube-polymer Interface[J]. Polym.,2003, 44(25): 7757 Fan Z, Hsiao KT, Advani SG. Experimental Investigation of Dispersion during Flow of Multi-walled Carbon Nanotube/Polymer Suspension in Fibrous Porous Media [J]. Carbon, 2004, 42: 871 Schadler LS, Giannaris SC, Ajayan PM. Load Transfer in Carbon Nanotube Epoxy Composites [J]. Appl. Phys. Lett.,1998, 73: 3842